The Accuracy of Characteristic Length Method on Failure Load Prediction of Composite Pinned Joints


 Marcus Eustace Whitehead
 1 years ago
 Views:
Transcription
1 , June 30  July 2, 2010, London, U.K. The Accuracy of Characteristic Length Method on Failure Load Prediction of Composite Pinned Joints O. Aluko, and Q. Mazumder Abstract An analytical model was developed to investigate the choice of failure criterion based on characteristic length method for predicting composite joint strength. The available experimental data for joint strength in literature were used to determine the accuracy of analytically obtained results. The analysis utilized six failure criteria, where it was shown that among the failure criteria investigated no one gave a best fit for all the three plates evaluated for strength, and the fit of individual failure theories is variable from one type of material to another. The results also showed that the accuracy of this method can be improved by computing the average predicted values of more than three failure criteria. Index Terms Characteristic length, Composite, Failure Criteria, and Joint strength. I. INTRODUCTION Adhesive bonding and mechanical bonding remain the two most common methods of joint design. While an adhesive joint offers the advantage of distributing the load over a larger area than a mechanical joint, its use is very restrictive due to its sensitivity to environmental conditions such as temperature and humidity. Therefore, mechanical joints are widely used as a reliable and practical method to assemble the composite parts that constitute a mechanical structure; they offer the advantage of assembly and disassembly for accessibility and maintenance, and reliability at various environmental conditions. However, a significant drawback when using the mechanical joint is that it always requires joint holes, which can be a source of stress concentration and thereby weakens the intended strength for the structures. Therefore, for the design of composite joints, stress and failure analysis around the fastener hole should first be conducted. During the loading of mechanical joints, the laminate deforms as the applied load increases and the contact surface between the fastener and the plate changes. It should be noted that despite the fact that the distributed stress around the fastener hole could be accurately determined, the failure at any point within the stress concentration region does not necessarily lead to failure of the joints. The strength of the structure will be underestimated if local failure is taken to be the ultimate failure of the joint. It becomes a big task to develop an analytic or computational method that can Manuscript submitted March 2, The Accuracy of Characteristic Length Method on Failure Load Prediction of Composite Pinned Joints. Olanrewaju Aluko is with the University of MichiganFlint, 303 E. Kearsley Street, Flint, MI USA (phone: ; fax: ; umflint.edu). Quamrul Mazumder., is with University of MichiganFlint, 303 E. Kearsley Street, Flint, MI 48502, USA. ( adequately model the complicated failure and structural response to loading of composite joints. Because of the complexity of the failure of composite joints coupled with the intension to reduce the cost and materials wastage in practical testing to failure, the analytical determination of bolted joint strength has received the attention of many researchers [1][16]. One of the most common and efficient methods of predicting the strength is the characteristic length method. This method was proposed by Whiney and Nuismer [1][3], and it has been further developed by Chang et. al [4]. For this improved method, both the characteristic lengths in tension, R t, and compression, R c, must be determined by stress analysis associated with the results of bearing and tensile tests on notched and unnotched plates before employing an appropriate failure theory along the characteristic curve, r c as shown in Figure 1. By definition, the characteristic length (in tension or compression) is the radial distance from the hole boundary over which the plate must be critically stressed to initiate a sufficient flaw that can cause failure. Wang et al. [5] analytically determined failure strength of composite joints in both circular and elliptical holes using stress functions developed by Lehknitskii [6] and TsaiWu failure criterion. However, only characteristic length in tension was used around the hole boundary to evaluate the failure load and mode of the composite joint. Whitworth et al. [7], [8] utilized the characteristic curve developed by Chang et. al [4] (which requires both the characteristic length in tension and compression to be determined) along with Yamada failure criterion to evaluate joint strength. Kweon et al. [9] developed a new method for finding the characteristic length in terms of arbitrarily applied loads, as an alternative to the failure load of notched plate in tension and bearing load of the plate when in compression. They evaluated the joint strength along the characteristic curve using TsaiWu failure criterion. In spite of the significant effort that has been invested on strength estimation of composite joints by various investigators using characteristic length method, the choice of an effective failure criterion in order to improve the accuracy of the characteristic dimensions remains to be investigated. For this paper, various failure criteria were utilized with the characteristic length method to predict the strength of composite joints with the objective to optimize the prediction accuracy of the characteristic length method. A twodimensional analysis which utilized stress functions for the computation of stresses at the hole boundary and within the plate was employed. In this investigation of the effective choice of failure criterion on the prediction accuracy of joint strength, six selected failure criteria based on the previous survey by Nahas [10] were utilized.
2 , June 30  July 2, 2010, London, U.K. II. CHARACTERICTIC LENGTHS METHOD As stated earlier, one of the most common and efficient methods of predicting joint strength is the characteristic length method. This study utilized the characteristic curve first proposed by Chang et al. [4], which requires both the characteristics length in tension, R t and compression, R c. These must be determined by stress analysis associated with the results of nobearing and tensile tests on notched and unnotched plates before employing an appropriate failure theory along the characteristic curve, r c as shown in Fig. 1. This characteristic curve which can be (1) where x and y are equal to r c cos θ and r c sin θ respectively. In this study, the plate (MO1) made from carbonepoxy unidirectional prepreg (USN125) and plain weave prepreg (HPW193) [11] with stacking sequence [±45 3 /90/±45 2 /0 4 /90/0 4 //±45 2 /90/±45 3 ] was used. The notation ±45 is used to represent a plane weave carbon/epoxy layer and the lamina thicknesses of the unidirectional and woven fabric layers are mm and 0.19 mm respectively. The hole diameter (d) is 9.53 mm, the width (W) of the plate is 26.8 mm, and the edge distance (e) is 19 mm. MO2 composite plate [9] was also utilized, having the same stacking sequence as above. The unidirectional layers are from the USN125 graphite/epoxy prepreg by Hankook Fiber Glass. The DMS2288 graphite/epoxy woven fabrics are by Sunkyong. The oneplythicknesses of the unidirectional and woven fabric layers are mm and mm, respectively. Other geometries of these two plates are the same. Additionally, AS4/ graphite/epoxy laminate having the stacking sequence [(45/0/45/0/90/0/45/0/45/0) 2 ] s with geometry of diameter (d), thickness (h), ratio of end distance to hole diameter (e/d) equal to cm, cm and 2, respectively was also used in this analysis [7]. The material properties of the three laminates are as given in Table I. a) Compressive characteristic length This analytical method employs the new approach proposed by Kweon et al. [9], without bearing tests to evaluate characteristic length in compression. This method utilizes any arbitrary load to compute the mean bearing stress, defined by: (2) where, P m, d and h are the arbitrary loads, diameter of hole and laminate thickness respectively. Within the context of this method, the compressive characteristic length R c as showed in Fig. 2 for point stress criterion [1] is the distance from the front holeedge to a point where the local compressive stress by the arbitrarily applied load is the same as the mean bearing stress. The present study utilized an analytical technique proposed by Aluko [12] to determine the compressive characteristic length. The analysis involved the stress functions that were computed from the displacement expressions that satisfy the boundary conditions. The semiinfinite plate in compression is as shown in Fig. 3. The boundary conditions of this geometry can be (3) (4) (5) where u and v are the displacements along x and y axes respectively. Therefore, the displacements u and v along the hole can be expressed by the following trigonometric series, (6) (7) where u 1, u 2, v 1 and v 2 are the unknowns to determine from boundary conditions. The condition of at free surface where x equal zero is: (8) Substituting (6) and (7) into (3), (4) and (5), we have Table I. The material properties of composite materials Propertie s Type of Material USN 125 HPW 193 DMS 2288 AS E 1 (GPa) E 2 (GPa) G 12 (GPa) υ X c (MPa) X t (MPa) Y c (MPa) Y t (MPa) S 12 (MPa) P m R c σ r =σ b d R t R c θ r c Characteristic curve Fig. 1. Schematic diagram for characteristic curve Fig. 2. Schematic diagram of the compressive characteristic length and normal stress distribution pattern
3 , June 30  July 2, 2010, London, U.K. θ y P Tensile stress distribution P R t Fig. 3. Schematic representation of compressive loading (9) The stress functions that satisfy the above displacement boundary conditions are [6]: (10) (11) However, the stresses in rectangular coordinate can be (12) Further, the stresses in polar coordinates can be obtained by stress transformations. In this model, frictionless condition is assumed between the pin and plate, Therefore, constant u o and c can be obtained from: (13) b) Tensile characteristic length x (14) Joints evaluation by the characteristic length method also requires the determination of tensile characteristic length. This involves the tensile test of notched (σ no) and unnotched (σ un ) laminate, as the strength values for the notched and unnotched laminates in tension must be known a priori. Fig. 4 shows the stress distribution of an infinite plate with a throughtothickness hole subjected to distributed tensile loads per unit area, P at infinity. The tensile stress would be highest at the side edges of the hole, and decreases further away from the side edges of the hole as shown in Fig. 4. In this analysis, the idea proposed by Konish and Whitney [13] for the approximate solution to the normal stress distribution σ y (x,0) in an infinite orthotropic plate with an open hole loaded in tension would be utilized. This solution can be (15) where the stress concentration factor K T and are expressed by the following: (16) (17) Tensile strength Fig. 4. Schematic diagram of the tensile characteristic length and stress distribution pattern where A ij, i,j = 1,2,6 denote the effective laminate inplane stiffness with 1 and 2 parallel and perpendicular to the loading direction respectively. The point stress criterion [2] can be applied to (15) to compute the tensile characteristic length at which failure analysis of the joint should be evaluated. The criterion defines the tensile characteristic length as the distance from the sideedge of the hole to a point where the tensile stress is the same as the strength of unnotched laminate. This can be (18) where, (19) The criterion assumes that the stress at infinity that determines the characteristic length defines the strength of the notched laminate. Substituting (17) and (18) into (15), the ratio of unnotched to notched strength is obtained as: (20) The value of tensile characteristic length can be determined if the data for tensile notched and unnotched laminate strength are known. The experimental values of notched and unnotched strength as obtained in the literature and the calculated values of both compressive and tensile characteristic length are shown in Table II. III. JOINT STRENGTH AND FAILURE ANALYSIS The present approach utilized an analytical technique that considers the orthotropic plate loaded with a force P by a rigid and frictionless pin (as shown in Fig. 5) to be homogeneous and infinite. In addition, the pin has the same diameter as the circular hole in the plate. Let the displacement of the plate due to pin load along x axis and at the ends of contact boundary be c o and c 1, respectively. Therefore, the boundary conditions of the geometry shown in Fig. 5 can be expressed as follows: (21) Table II: Characteristic length and strength data for the plates Plate R c, m R t, m Notched strength, MPa Unnotched strength, MPa MO MO AS
4 , June 30  July 2, 2010, London, U.K. (22) (23) where u and v are the displacements along x and y axes respectively. The condition for no contact surface can be (24) (25) Using (6) and (7) to satisfy the above displacement boundary conditions, we calculated the unknown u i and v i to be: (26a) (26b) The stress functions that satisfy the above displacement boundary conditions are [6]: (35) The prime implies the derivative of the stress functions. The parameters c o and c 1 can be determined from material properties of the plate and the condition of traction at the hole boundary. The traction for the case frictionless condition can be (36) (37) (27a) (38a) (27b) The stresses in rectangular coordinates can be expressed as [6]: (28a) (28b) (28c) where bar implies conjugate and (29) (30) (31) (32) (33) with a ij, i,j =1,2,6 are the compliances, and μ 1 and μ 2 are the roots of characteristics equation for orthotropic plate defined by: (34) where 1 and 2 are parallel and transverse to the loading direction, respectively, and r is the radius of the hole. The stresses in polar coordinates are given by the expressions: x Fig. 5. Schematic representation of composite joint P θ y (38b) Parameters k, n and g are materials constant of the plate (40) The stress results computed from above analytical method along the characteristic curve (shown in Fig. 1) were used in failure analysis to predict the joint strength for first ply failure. In an attempt to increase the accuracy of joint strength prediction by characteristic length method, six failure criteria based on the previous survey by Nahas [10] were used in conjunction with characteristic dimensions for the evaluation. In his survey, Nahas referenced the previous study by Burk [15] stating that AzziTsai and TsaiWu are among the four most commonly used failure criteria. Nahas also referenced the work of Owen and Rice [16] that asserts Fischer theory provides the best overall fit for static test results. The various failure criteria utilized in this analysis include the following [10]: YamadaSun: (41) AzziTsai: (42) Fisher: TsaiWu: (43) (44) Norris: (45) NorrisMckinnon: (46) Where σ 1 and σ 2 are longitudinal stresses and τ 12 is shear stress, X and Y are the ply longitudinal strength and S the ply shear strength. In this model, failure is expected to occur when the above equations are met. The computer code used to test for the condition of failure was written in Mathematica. The concept of finitewidth correction factor developed by Tan [14] was utilized to correct the infinite assumption of the plate. By definition, finitewidth correction factor (FWC) is a scale factor which is applied to multiply the notched infinite plate solution to obtain the notched
5 , June 30  July 2, 2010, London, U.K. finiteplate result based on the assumption that the normal stress profile for a finite plate is identical to that for an infinite except for a FWC factor. This correction factor is given by the relationship: (47) K T /K T is the FWC factor and K T and K T denote the stress concentration at the opening edge on the axis normal to the applied load for a finite plate and an infinite plate, respectively. The parameters σ N and are the failure strength of finitewidth and infinite plates, respectively. This factor is expressed by the relationship [14]: (48) where r is the radius of the hole and w defines the width of the plate. IV. RESULTS AND DISCUSSION The failure loads computed from the above analysis with failure criteria and their percentage differences with the experimentally obtained value for three different composite plates are shown in Table III. It can be seen from this table that no criterion provided the best fit for all the plate evaluated, and the fit of individual failure theories is variable from one type of material to another. Documented in Fig. 6 is the predicted load for MO1 plate as compared with experimental value. Due to variability in material properties, the experimental value for this plate [11] varies between 11.3 and 13.0 kn, which can be approximated to ±7.13% over the mean value. It can be depicted from this figure that all the predictions except TsaiWu which over estimated the strength are suitable for this plate. Keweon et al. [9] showed that seven specimens were tested for plate MO2 and the computed coefficient of variation (defined as standard deviation over the mean failure load) was equal to 6.1 percent. Even though the range for the experimental failure load cannot be computed from the coefficient of variation, it is evident from Fig. 7 that Fisher criterion is not an adequate predictor of strength. Therefore, the conclusion reached by Owen and Rice [16] that the Fisher theory provides the best overall fit for static tests results does not apply to all plates, as shown in this figure. Fisher theory severely underestimated the failure strength for MO2 plate. For AS plate, no information with regard to material variability was given. Notwithstanding, all the various criteria employed in this study appear to be adequate for the plate as documented in Fig. 8, with Fisher criterion yielding the best prediction. It should be noted that while TsaiWu failure theory over estimates the failure strength for all the three plates evaluated, the calculated average values of each prediction give a better fit for all the plates. V. CONCLUSION Stress analysis was performed to predict failure strength of pin loaded composite joints using the six failure criteria and on ChangScottSpringer characteristic curve model. The characteristic length in compression and tension that defines the characteristic curve was obtained by stress analysis associated with no bearing test and tensile test on laminate with and without a hole. The available experimental data in literature for different laminated composites were used to evaluate the joints strength. The agreement between Table III: Predicted loads and the percentage difference between experimental values Failure criteria MO1 (kn) MO2 ( kn) AS ( kn) MO1 (%) MO2 (%) AS (%) Experiment Yamada Sun AzziTs ai Norrs Mckinn on Norris Fisher TsaiW u Average Fig. 6: Failure predictions for MO1 Plate, [±45 3 /90/±45 2 /0 4 /90/0 4 //±45 2 /90/±45 3 ] Fig.7: Failure predictions for MO2 plate, [±45 3 /90/±45 2 /0 4 /90/0 4 //±45 2 /90/±45 3 ] experimental bearing strength for three different laminated composite plates evaluated and the analytically obtained joint strength by characteristic length method for each depends on the choice of failure criterion.
6 , June 30  July 2, 2010, London, U.K. Fig. 8: Failure predictions for AS Plate, [(45/0/45/0/90/0/45/0/45/0) 2 ] s There is no single failure criterion provided the best fit for all the plates evaluated; the average value of the predicted results from the six failure criteria investigated showed close agreement. Therefore, in order to optimize the accuracy of characteristic length method for joint strength prediction, three or more failure theories must be employed and an average calculated. REFERENCES [1] R.J. Nuismer, 1979, Application of the average stress failure criterion: Part II  Compression, Journal of composite materials, 13, pp [2] J.M. Whitney, and R.J. Nuismer, 1974, Stress fracture criteria for laminated composites containing stress concentrations, Journal of composite materials, 8 (253), pp [3] J.M. Whitney, and R.J. Nuismer, 1975, Uniaxial failure of composite laminated containing stress concentrations, Fracture mechanics of composite, ASTM STP, pp [4] F.K. Chang, and R.A. Scott, 1982, Strength of mechanically fastened composite joints, Journal of composite materials, 16, pp [5] J.T. Wang, C.G. Lotts, and D.D. Davis, Analysis of boltloaded elliptical holes in laminated composite joints. Journal of reinforced plastics and composites 1985;12: [6] Lekhnitskii, S.G., 1968, Anisotropic plates, Translated from the 2 nd Russian edition by S.W. Tsai, and T. Chevron, Gordon and Breach, London [7] H. A. Whitworth, M. Othieno, and O. Barton, 2003, Failure analysis of composite pin loaded joints, Composite structures, 59, pp [8] H. A. Whitworth, O. Aluko, and N.A. Tomlinson, 2008, Application of point stress criterion to the failure of composite pinned joints, Engineering fracture mechanics, 75, pp [9] J. Kweon, H. Ahn, and J. Choi, 2004, A new method to determine the characteristic lengths of composite joints without testing, Composite structures, 66, pp [10] M.N. Nahas, 1986, Survey of failure and postfailure theories of laminated fiberreinforced composites, Journal of composites technology and research, 8(4), pp [11] J. Choi, and Y. Chun, 2003, Failure load prediction of mechanically fastened composite joints, Journal of composite materials, 37(24), pp [12] O. Aluko, 2009, Analytic determination of compressive characteristic length of composite plate, Early career journal, ASME 8, pp [13] J.H. Konish, and J.M. Whitney, 1975, Approximate stresses in an orthotropic plate containing a circular hole, Journal of composite materials, 9, pp [14] S.C. Tan, 1988, Finitewidth correction factors for anisotropic plate containing a central opening, Journal of composite materials, 22, pp [15] R.C. Burk, 1983, Standard failure criteria needed for advanced composites, astronautics and aeronautics, 22, pp [16] M.J. Owen, and D.J. Rice, 1981, Biaxial strength behavior of glass fabricreinforced polyester resin, composites, 12, pp
Failure analysis of serial pinned joints in composite materials
Indian Journal of Engineering & Materials Sciences Vol. 18, April 2011, pp. 102110 Failure analysis of serial pinned joints in composite materials Alaattin Aktaş* Department of Mechanical Engineering,
More informationNUMERICAL MODELLING OF COMPOSITE PIN JOINTS AND EXPERIMENTAL VALIDATION
NUMERICAL MODELLING OF COMPOSITE PIN JOINTS AND EXPERIMENTAL VALIDATION Fabrice PIERRON*, François CERISIER*, and Michel GRÉDIAC** * SMS/ Département Mécanique et Matériaux, École Nationale Supérieure
More informationACDC. User Manual. Ver. 1.0
ACDC User Manual Ver. 1.0 Centre Composite December 2016 ACDC, Ver. 1.0 User Manual Centre Composite, 2016 (software@composite.lv) Table of Contents Introduction... 1 System requirements... 1 Theoretical
More informationOpenhole compressive strength prediction of CFRP composite laminates
Openhole compressive strength prediction of CFRP composite laminates O. İnal 1, A. Ataş 2,* 1 Department of Mechanical Engineering, Balikesir University, Balikesir, 10145, Turkey, inal@balikesir.edu.tr
More informationthe failure strengths and failure modes of composite laminates containing
464 Failure Strength of Nonlinearly Elastic Composite Laminates Containing a Pin Loaded Hole FUKUO CHANG AND RICHARD A. SCOTT Department of Mechanical Engineering and Applied Mechanics The University
More informationQUESTION BANK Composite Materials
QUESTION BANK Composite Materials 1. Define composite material. 2. What is the need for composite material? 3. Mention important characterits of composite material 4. Give examples for fiber material 5.
More informationBIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS
BIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS H. Kumazawa and T. Takatoya Airframes and Structures Group, Japan Aerospace Exploration Agency 6131, Ohsawa, Mitaka,
More informationFailure Analysis of Unidirectional Composite Pinned Joints
217 IJEDR Volume, Issue 4 ISSN: 23219939 Failure Analysis of Unidirectional Composite Pinned Joints 1 Sai Ashok.M, 2 Mr. U. Koteswara Rao 1 Mtech Machine Design, 2 Associate Professor & Asst. COE 1
More informationDerivation of the stress concentrations at holes in orthotropic plates using thermoelastic stress analysis
Derivation of the stress concentrations at holes in orthotropic plates using thermoelastic stress analysis S. Quinn, S. Sambasivam and J.M. DulieuBarton School of Engineering Sciences, University of Southampton,
More informationModule III  Macromechanics of Lamina. Lecture 23. MacroMechanics of Lamina
Module III  Macromechanics of Lamina Lecture 23 MacroMechanics of Lamina For better understanding of the macromechanics of lamina, the knowledge of the material properties in essential. Therefore, the
More informationMODELING OF THE BEHAVIOR OF WOVEN LAMINATED COMPOSITES UNTIL RUPTURE
MODELING OF THE BEHAVIOR OF WOVEN LAMINATED COMPOSITES UNTIL RUPTURE Jean Paul Charles, Christian Hochard,3, Pierre Antoine Aubourg,3 Eurocopter, 375 Marignane cedex, France Unimeca, 6 rue J. Curie, 3453
More informationStrength of GRPlaminates with multiple fragment damages
Strength of GRPlaminates with multiple fragment damages S. Kazemahvazi, J. Kiele, D. Zenkert Kungliga Tekniska Högskolan, KTH 100 44 Stockholm, Sweden sohrabk@kth.se SUMMARY The strength of glass fibre
More informationME 7502 Lecture 2 Effective Properties of Particulate and Unidirectional Composites
ME 75 Lecture Effective Properties of Particulate and Unidirectional Composites Concepts from Elasticit Theor Statistical Homogeneit, Representative Volume Element, Composite Material Effective Stress
More informationFracture Mechanics, Damage and Fatigue: Composites
University of Liège Aerospace & Mechanical Engineering Fracture Mechanics, Damage and Fatigue: Composites Ludovic Noels Computational & Multiscale Mechanics of Materials CM3 http://www.ltascm3.ulg.ac.be/
More informationINTERNATIONAL JOURNAL OF APPLIED ENGINEERING RESEARCH, DINDIGUL Volume 2, No 1, 2011
Interlaminar failure analysis of FRP cross ply laminate with elliptical cutout Venkateswara Rao.S 1, Sd. Abdul Kalam 1, Srilakshmi.S 1, Bala Krishna Murthy.V 2 1 Mechanical Engineering Department, P. V.
More informationComputational Analysis for Composites
Computational Analysis for Composites Professor Johann Sienz and Dr. Tony Murmu Swansea University July, 011 The topics covered include: OUTLINE Overview of composites and their applications Micromechanics
More informationStress, Strain Stress strain relationships for different types of materials Stress strain relationships for a unidirectional/bidirectional lamina
Chapter 2 Macromechanical Analysis of a Lamina Stress, Strain Stress strain relationships for different types of materials Stress strain relationships for a unidirectional/bidirectional lamina Islamic
More informationDAMAGE MECHANICS MODEL FOR OFFAXIS FATIGUE BEHAVIOR OF UNIDIRECTIONAL CARBON FIBERREINFORCED COMPOSITES AT ROOM AND HIGH TEMPERATURES
DAMAGE MECHANICS MODEL FOR OFFAXIS FATIGUE BEHAVIOR OF UNIDIRECTIONAL CARBON FIBERREINFORCED COMPOSITES AT ROOM AND HIGH TEMPERATURES M. Kawai Institute of Engineering Mechanics University of Tsukuba,
More informationMechanical Behavior of Circular Composite Springs with Extended Flat Contact Surfaces
Mechanical Behavior of Circular Composite Springs with Extended Flat Contact Surfaces PingCheung Tse epartment of Mechanical Engineering, The Hong Kong Polytechnic University, Hunghom, Kowloon, Hong Kong
More informationTABLE OF CONTENTS. Mechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA
Mechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA TABLE OF CONTENTS 1. INTRODUCTION TO COMPOSITE MATERIALS 1.1 Introduction... 1.2 Classification... 1.2.1
More informationIJSER 1. INTRODUCTION. M.Elhadary
1591 A new failure criterion for GRP composite materials subjected to inphase and outofphase biaxial fatigue loading under different stress ratios M.Elhadary Abstract this studying the fatigue behavior
More informationME 582 Advanced Materials Science. Chapter 2 Macromechanical Analysis of a Lamina (Part 2)
ME 582 Advanced Materials Science Chapter 2 Macromechanical Analysis of a Lamina (Part 2) Laboratory for Composite Materials Research Department of Mechanical Engineering University of South Alabama, Mobile,
More informationA NEW STRENGTH TENSOR BASED FAILURE CRITERION FOR ANISOTROPIC MATERIALS
A NEW STRENGTH TENSOR BASED FAILURE CRITERION FOR ANISOTROPIC MATERIALS Paul V. Osswald, Technical University of Munich, Munich, Germany Tim A. Osswald, Polymer Engineering Center, University of WisconsinMadison,
More informationCalculation of Damagedependent Directional Failure Indices from the TsaiWu Static Failure Criterion
Van Paepegem, W. and Degrieck, J. (3. alculation of Damagedependent Directional Failure Indices from the saiwu Static Failure riterion. omposites Science and echnology, 63(, 353. alculation of Damagedependent
More informationTHE ROLE OF DELAMINATION IN NOTCHED AND UNNOTCHED TENSILE STRENGTH
THE ROLE OF DELAMINATION IN NOTCHED AND UNNOTCHED TENSILE STRENGTH M. R. Wisnom University of Bristol Advanced Composites Centre for Innovation and Science University Walk, Bristol BS8 1TR, UK M.Wisnom@bristol.ac.uk
More informationCHAPTER 6 MECHANICAL PROPERTIES OF METALS PROBLEM SOLUTIONS
CHAPTER 6 MECHANICAL PROPERTIES OF METALS PROBLEM SOLUTIONS Concepts of Stress and Strain 6.1 Using mechanics of materials principles (i.e., equations of mechanical equilibrium applied to a freebody diagram),
More informationFinite element modelling of infinitely wide Angleply FRP. laminates
www.ijaser.com 2012 by the authors Licensee IJASER Under Creative Commons License 3.0 editorial@ijaser.com Research article ISSN 2277 9442 Finite element modelling of infinitely wide Angleply FRP laminates
More informationTensile behaviour of antisymmetric CFRP composite
Available online at www.sciencedirect.com Procedia Engineering 1 (211) 1865 187 ICM11 Tensile behaviour of antisymmetric CFRP composite K. J. Wong a,b, *, X. J. Gong a, S. Aivazzadeh a, M. N. Tamin b
More informationComparison of Plywise StressStrain results for graphite/epoxy laminated plate subjected to inplane normal loads using CLT and ANSYS ACP PrepPost
Comparison of Plywise StressStrain results for graphite/epoxy laminated plate subjected to inplane normal loads using CLT and ANSYS ACP PrepPost 1 Mihir A. Mehta, 2 Satyen D. Ramani 1 PG Student, Department
More informationRELATIONSHIP BETWEEN RADIAL COMPRESSIVE MODULUS OF ELASTICITY AND SHEAR MODULUS OF WOOD Jen Y. Liu Research Engineer
RELATIONSHIP BETWEEN RADIAL COMPRESSIVE MODULUS OF ELASTICITY AND SHEAR MODULUS OF WOOD Jen Y. Liu Research Engineer and Robert J. Ross Supervisory Research Engineer USDA Forest Service Forest Products
More informationCapability Assessment of Finite Element Software in Predicting the Last Ply Failure of Composite Laminates
Available online at www.sciencedirect.com Procedia Engineering 41 (2012 ) 1647 1653 International Symposium on Robotics and Intelligent Sensors 2012 (IRIS 2012) Capability Assessment of Finite Element
More informationMechanics of Earthquakes and Faulting
Mechanics of Earthquakes and Faulting Lectures & 3, 9/31 Aug 017 www.geosc.psu.edu/courses/geosc508 Discussion of Handin, JGR, 1969 and Chapter 1 Scholz, 00. Stress analysis and Mohr Circles Coulomb Failure
More informationNonconventional Glass fiber NCF composites with thermoset and thermoplastic matrices. F Talence, France Le Cheylard, France
20 th International Conference on Composite Materials Copenhagen, 1924th July 2015 Nonconventional Glass fiber NCF composites with thermoset and thermoplastic matrices. Thierry Lorriot 1, Jalal El Yagoubi
More informationBEARING STRENGTH ASSESSMENT OF COMPOSITE MATERIAL THROUGH NUMERICAL MODELS
BEARING STRENGTH ASSESSMENT OF COMPOSITE MATERIAL THROUGH NUMERICAL MODELS Euler S. Dias*, Carlos A. Cimini Jr.* * Federal University of Minas Gerais, Dept. of Structural Engineering, Belo Horizonte 
More informationDevelopment of a Progressive Failure Model for Notched Woven Composite Laminates. Daniel Christopher Munden
Development of a Progressive Failure Model for Notched Woven Composite Laminates Daniel Christopher Munden Thesis submitted to the faculty of the Virginia Polytechnic Institute and State University in
More informationStress intensity factors for an inclined and/or eccentric crack in a finite orthotropic lamina
1886 Stress intensity factors for an inclined and/or eccentric crack in a finite orthotropic lamina Abstract Stress intensity factors (SIF) are determined for an inclined and / or eccentric crack in a
More informationInfluence of the filament winding process variables on the mechanical behavior of a composite pressure vessel
Influence of the filament winding process variables on the mechanical behavior of a composite pressure vessel G. Vargas 1 & A. Miravete 2 1 Universidad Pontificia Bolivariana, Facultad de Ingeniería Mecánica,
More informationAnalysis of Composite Pressure Vessels
Analysis of Composite Pressure Vessels Reza Mohammadzadeh Gheshlaghi 1 Mohammad Hassan Hojjati Hamid Reza Mohammadi Daniali 3 1 Engineering Research Centre, Tabriz, Iran,3 Department of Mechanical Engineering,
More informationNumerical investigation on the position of holes for reducing stress concentration in composite plates with bolted and riveted joints
THEORETICAL & APPLIED MECHANICS LETTERS 1, 041005 (2011) Numerical investigation on the position of holes for reducing stress concentration in composite plates with bolted and riveted joints M. R. Khoshravan,
More informationGeometric and Material Property Effects on the Strength of RubberToughened Adhesive Joints
Geometric and Material Property Effects on the Strength of RubberToughened Adhesive Joints Altering the geometry of a bonded joint will invariably cause changes to occur in the stress and strain distribution
More informationNotched Strength Estimation of Graphite/Epoxy Laminated Composite with Central Crack under Uniaxial Tensile Loading
International Journal o Composite Materials 5, 5(6): 778 DOI:.593/j.cmaterials.556.6 Notched Strength Estimation o Graphite/Epoxy Laminated Composite with Central Crack under Uniaxial Tensile Loading
More informationDYNAMIC FAILURE ANALYSIS OF LAMINATED COMPOSITE PLATES
Association of Metallurgical Engineers of Serbia AMES Scientific paper UDC:669.1419:628.183=20 DYNAMIC FAILURE ANALYSIS OF LAMINATED COMPOSITE PLATES J. ESKANDARI JAM 1 and N. GARSHASBI NIA 2 1 Aerospace
More informationPRELIMINARY PREDICTION OF SPECIMEN PROPERTIES CLT and 1 st order FEM analyses
OPTIMAT BLADES Page 1 of 24 PRELIMINARY PREDICTION OF SPECIMEN PROPERTIES CLT and 1 st order FEM analyses first issue Peter Joosse CHANGE RECORD Issue/revision date pages Summary of changes draft 241002
More informationMECHANICAL FAILURE OF A COMPOSITE HELICOPTER STRUCTURE UNDER STATIC LOADING
MECHANICAL FAILURE OF A COMPOSITE HELICOPTER STRUCTURE UNDER STATIC LOADING Steven Roy, Larry Lessard Dept. of Mechanical Engineering, McGill University, Montreal, Québec, Canada ABSTRACT The design and
More informationEffect of Thermal Stresses on the Failure Criteria of Fiber Composites
Effect of Thermal Stresses on the Failure Criteria of Fiber Composites Martin Leong * Institute of Mechanical Engineering Aalborg University, Aalborg, Denmark Bhavani V. Sankar Department of Mechanical
More informationPractice Final Examination. Please initial the statement below to show that you have read it
EN175: Advanced Mechanics of Solids Practice Final Examination School of Engineering Brown University NAME: General Instructions No collaboration of any kind is permitted on this examination. You may use
More informationNUMERICAL FEM ANALYSIS FOR THE PART OF COMPOSITE HELICOPTER ROTOR BLADE
Journal of KONES Powertrain and Transport, Vol. 19, No. 1 2012 NUMERICAL FEM ANALYSIS FOR THE PART OF COMPOSITE HELICOPTER ROTOR BLADE Hubert D bski Lublin University of Technology, Department of Machine
More informationInternational Journal of Innovative Research in Science, Engineering and Technology Vol. 2, Issue 7, July 2013
ANALYSIS AND MITIGATION OF STRESS CONCENTRATION FACTOR OF A RECTANGULAR ISOTROPIC AND ORTHOTROPIC PLATE WITH CENTRAL CIRCULAR HOLE SUBJECTED TO INPLANE STATIC LOADING BY DESIGN OPTIMIZATION Shubhrata Nagpal
More informationHygrothermal stresses in laminates
Hygrothermal stresses in laminates Changing environment conditions (temperature and moisture) have an important effect on the properties which are matrix dominated. Change in temperaturet and moisture
More informationMULTISCALE AND MULTILEVEL ANALYSIS OF COMPOSITE STRUCTURES WITH BOLTED JOINTS
MULTISCALE AND MULTILEVEL ANALYSIS OF COMPOSITE STRUCTURES WITH BOLTED JOINTS F.X. Irisarri, J.F. Maire* and N. Carrere ONERA, 9 av. de la Division Leclerc, 930 Châtillon, France francoisxavier.irisarri@onera.fr,
More informationMechanical Properties of Materials
Mechanical Properties of Materials Strains Material Model Stresses Learning objectives Understand the qualitative and quantitative description of mechanical properties of materials. Learn the logic of
More informationEVALUATION OF DAMAGE DEVELOPMENT FOR NCF COMPOSITES WITH A CIRCULAR HOLE BASED ON MULTISCALE ANALYSIS
THE 19 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS EVALUATION OF DAMAGE DEVELOPMENT FOR NCF COMPOSITES WITH A CIRCULAR HOLE BASED ON MULTISCALE ANALYSIS T. Kurashiki 1 *, Y. Matsushima 1, Y. Nakayasu
More informationELASTICITY AND FRACTURE MECHANICS. Vijay G. Ukadgaonker
THEORY OF ELASTICITY AND FRACTURE MECHANICS y x Vijay G. Ukadgaonker Theory of Elasticity and Fracture Mechanics VIJAY G. UKADGAONKER Former Professor Indian Institute of Technology Bombay Delhi110092
More informationPREDICTION OF OUTOFPLANE FAILURE MODES IN CFRP
PREDICTION OF OUTOFPLANE FAILURE MODES IN CFRP R. R. Pinto 1, P. P. Camanho 2 1 INEGI  Instituto de Engenharia Mecanica e Gestao Industrial, Rua Dr. Roberto Frias, 4200465, Porto, Portugal 2 DEMec,
More informationChapter 2  Macromechanical Analysis of a Lamina. Exercise Set. 2.1 The number of independent elastic constants in three dimensions are: 2.
Chapter  Macromechanical Analysis of a Lamina Exercise Set. The number of independent elastic constants in three dimensions are: Anisotropic Monoclinic 3 Orthotropic 9 Transversely Orthotropic 5 Isotropic.
More informationTHREE DIMENSIONAL STRESS ANALYSIS OF THE T BOLT JOINT
THREE DIMENSIONAL STRESS ANALYSIS OF THE T BOLT JOINT Víctor Martínez 1, Alfredo Güemes 2, Norbert Blanco 1, Josep Costa 1 1 Escola Politècnica Superior. Universitat de Girona. Girona, Spain (17071) 2
More informationModelling the nonlinear shear stressstrain response of glass fibrereinforced composites. Part II: Model development and finite element simulations
Modelling the nonlinear shear stressstrain response of glass fibrereinforced composites. Part II: Model development and finite element simulations W. Van Paepegem *, I. De Baere and J. Degrieck Ghent
More informationSINGLEBOLTED CONNECTIONS FOR ORTHOTROPIC FIBREREINFORCED COMPOSITE STRUCTURAL MEMBERS
SINGLEBOLTED CONNECTIONS FOR ORTHOTROPIC FIBREREINFORCED COMPOSITE STRUCTURAL MEMBERS BY CHARLES N. ROSNER A Thesis Submitted to the Faculty of Graduate Studies in Partial Fulfilment of the Requirements
More informationInfluence of fibre proportion and position on the machinability of GFRP composites An FEA model
Indian Journal of Engineering & Materials Sciences Vol. 12, October 2005, pp. 443450 Influence of fibre proportion and position on the machinability of GFRP composites An FEA model D Abdul Budan* Department
More information[5] Stress and Strain
[5] Stress and Strain Page 1 of 34 [5] Stress and Strain [5.1] Internal Stress of Solids [5.2] Design of Simple Connections (will not be covered in class) [5.3] Deformation and Strain [5.4] Hooke s Law
More informationStrength Prediction Of Composite Laminate
Strength Prediction Of Composite te Prof. Yogananda. A 1, Mr. R. Vijayakumar 2 Assistant Professor, Department of Mechanical Engineering, East West Institute of Technology, Bangalore. Research Scholar,
More informationMechanical analysis of timber connection using 3D finite element model
Mechanical analysis of timber connection using 3D finite element model Bohan XU Ph.D Student Civil Engineering Laboratory (CUST) ClermontFerrand, France Mustapha TAAZOUNT DrIng Civil Engineering Laboratory
More informationMultiscale Approach to Damage Analysis of Laminated Composite Structures
Multiscale Approach to Damage Analysis of Laminated Composite Structures D. Ivančević and I. Smojver Department of Aeronautical Engineering, Faculty of Mechanical Engineering and Naval Architecture, University
More informationSTRESS DISTRIBUTION AND STRENGTH PREDICTION OF COMPOSITE LAMINATES WITH MULTIPLE HOLES BRIAN ESP. Presented to the Faculty of the Graduate School of
STRESS DISTRIBUTION AND STRENGTH PREDICTION OF COMPOSITE LAMINATES WITH MULTIPLE HOLES by BRIAN ESP Presented to the Faculty of the Graduate School of The University of Texas at Arlington in Partial Fulfillment
More informationMechanics of Earthquakes and Faulting
Mechanics of Earthquakes and Faulting www.geosc.psu.edu/courses/geosc508 Surface and body forces Tensors, Mohr circles. Theoretical strength of materials Defects Stress concentrations Griffith failure
More informationCOMPARISON OF NUMERICAL SIMULATION AND EXPERIMENT OF A FLEXIBLE COMPOSITE CONNECTING ROD
10th International DAAAM Baltic Conference "INDUSTRIAL ENGINEERING  1213 May 2015, Tallinn, Estonia COMPARISON OF NUMERICAL SIMULATION AND EXPERIMENT OF A FLEXIBLE COMPOSITE CONNECTING ROD Sedláček,
More informationEffects of Resin and Fabric Structure
Fatigue of Wind Blade Laminates: Effects of Resin and Fabric Structure Details David Miller, Daniel D. Samborsky and John F. Mandell Montana State t University it MCARE 2012 Outline Overview of MSU Fatigue
More informationCalculation of Energy Release Rate in Mode I Delamination of Angle Ply Laminated Composites
Copyright c 2007 ICCES ICCES, vol.1, no.2, pp.6167, 2007 Calculation of Energy Release Rate in Mode I Delamination of Angle Ply Laminated Composites K. Gordnian 1, H. Hadavinia 1, G. Simpson 1 and A.
More informationRATEDEPENDENT OFFAXIS COMPRESSIVE STRENGTH OF A UNIDIRECTIONAL CARBON/EPOXY LAMINATE AT HIGH TEMPERATURE
16 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS RATEDEPENDENT OFFAXIS COMPRESSIVE STRENGTH OF A UNIDIRECTIONAL CARBON/EPOXY LAMINATE AT HIGH TEMPERATURE Masamichi KAWAI *, Satoru SAITO **, JianQi
More informationEnhancing Prediction Accuracy In Sift Theory
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS Enhancing Prediction Accuracy In Sift Theory J. Wang 1 *, W. K. Chiu 1 Defence Science and Technology Organisation, Fishermans Bend, Australia, Department
More informationPREDICTION OF BUCKLING AND POSTBUCKLING BEHAVIOUR OF COMPOSITE SHIP PANELS
FONDATĂ 1976 THE ANNALS OF DUNAREA DE JOS UNIVERSITY OF GALATI. FASCICLE IX. METALLURGY AND MATERIALS SCIENCE N 0. 007, ISSN 15 08X PREDICTION OF BUCKLING AND POSTBUCKLING BEHAVIOUR OF COMPOSITE SHIP PANELS
More informationMechanics of Materials Primer
Mechanics of Materials rimer Notation: A = area (net = with holes, bearing = in contact, etc...) b = total width of material at a horizontal section d = diameter of a hole D = symbol for diameter E = modulus
More informationAn investigation of the mechanical behaviour of carbon epoxy cross ply cruciform specimens under biaxial loading
An investigation of the mechanical behaviour of carbon epoxy cross ply cruciform specimens under biaxial loading A. Makris, C. Ramault, D. Van Hemelrijck Department of Mechanics of Materials and Constructions,
More informationPLY LEVEL UNCERTAINTY EFFECTS ON FAILURE OF COMPOSITE
7th European Workshop on Structural Health Monitoring July 811, 2014. La Cité, Nantes, France More Info at Open Access Database www.ndt.net/?id=17206 PLY LEVEL UNCERTAINTY EFFECTS ON FAILURE OF COMPOSITE
More informationFinite element analysis of bolted connections for PFRP composites
13598368(95)000461 Composites: Part B 278 (1996) 339349 Copyright 1:1) 1996 Elsevier Science Limited Printed in Great Britain. All rights reserved 13598568/96/$15.00 Finite element analysis of bolted
More informationLAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS
XXII. LAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS Introduction The lamination theory for the elastic stiffness of fiber composite materials is the backbone of the entire field, it holds
More informationEXPLICIT DYNAMIC SIMULATION OF DROPWEIGHT LOW VELOCITY IMPACT ON CARBON FIBROUS COMPOSITE PANELS
EXPLICIT DYNAMIC SIMULATION OF DROPWEIGHT LOW VELOCITY IMPACT ON CARBON FIBROUS COMPOSITE PANELS Umar Farooq and Karl Gregory School of Built Environment and Department of Engineering, University of Bolton,
More informationModeling and Simulations of Aircraft Structures Stiffness, Damage, and Failure Prediction for Laminated Composites
Modeling and Simulations of Aircraft Structures Stiffness, Damage, and Failure Prediction for Laminated Composites H.E.Pettermann 1, C.Schuecker 1, D.H.Pahr 2, F.G.Rammerstorfer 2 1 Austrian Aeronautics
More informationS HEAR S TRENGTH IN P RINCIPAL P LANE OF W OOD
S HEAR S TRENGTH IN P RINCIPAL P LANE OF W OOD By Jen Y. Liu 1 and Lester H. Floeter 2 ABSTRACT: In this study, the writers used Tsai and Wu s tensor polynomial theory to rederive a formula originally
More informationCHEMC2410: Materials Science from Microstructures to Properties Composites: basic principles
CHEMC2410: Materials Science from Microstructures to Properties Composites: basic principles Mark Hughes 14 th March 2017 Today s learning outcomes To understand the role of reinforcement, matrix and
More informationDAMAGE SIMULATION OF CFRP LAMINATES UNDER HIGH VELOCITY PROJECTILE IMPACT
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS DAMAGE SIMULATION OF CFRP LAMINATES UNDER HIGH VELOCITY PROJECTILE IMPACT A. Yoshimura 1*, T. Okabe, M. Yamada 3, T. Ogasawara 1, Y. Tanabe 3 1 Advanced
More informationStandard Test Method for Open Hole Tensile Strength of Polymer Matrix Composite Laminates 1
This document is not an ASTM standard and is intended only to provide the user of an ASTM standard an indication of what changes have been made to the previous version. Because it may not be technically
More information3.2.2 principal material coordinate system, n a coordinate system with axes that are normal to the planes of symmetry inherent to a material
Designation: Standard Test Method for Open Hole Tensile Strength of Polymer Matrix Composite Laminates 1 This standard is issued under the fixed designation D 5766/D 5766M; the number immediately following
More informationGetting Started with Composites Modeling and Analysis
Getting Started with Composites Modeling and Analysis IN THIS WEBINAR: PRESENTED BY: Orthotropic materials and how to define them Composite Laminate properties and modeling Composite failure theories and
More informationThe University of Melbourne Engineering Mechanics
The University of Melbourne 436291 Engineering Mechanics Tutorial Four Poisson s Ratio and Axial Loading Part A (Introductory) 1. (Problem 922 from Hibbeler  Statics and Mechanics of Materials) A short
More informationTHE MUTUAL EFFECTS OF SHEAR AND TRANSVERSE DAMAGE IN POLYMERIC COMPOSITES
THE 19 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS THE MUTUAL EFFECTS OF SHEAR AND TRANSVERSE DAMAGE IN POLYMERIC COMPOSITES L.V. Smith 1 *, M. Salavatian 1 1 School of Mechanical and Materials
More informationCHAPTER 3 THE EFFECTS OF FORCES ON MATERIALS
CHAPTER THE EFFECTS OF FORCES ON MATERIALS EXERCISE 1, Page 50 1. A rectangular bar having a crosssectional area of 80 mm has a tensile force of 0 kn applied to it. Determine the stress in the bar. Stress
More informationUNIT I SIMPLE STRESSES AND STRAINS
Subject with Code : SM1(15A01303) Year & Sem: IIB.Tech & ISem SIDDHARTH GROUP OF INSTITUTIONS :: PUTTUR Siddharth Nagar, Narayanavanam Road 517583 QUESTION BANK (DESCRIPTIVE) UNIT I SIMPLE STRESSES
More informationExercise: concepts from chapter 8
Reading: Fundamentals of Structural Geology, Ch 8 1) The following exercises explore elementary concepts associated with a linear elastic material that is isotropic and homogeneous with respect to elastic
More informationMECHANICS OF MATERIALS
Third E CHAPTER 1 Introduction MECHANICS OF MATERIALS Ferdinand P. Beer E. Russell Johnston, Jr. John T. DeWolf Lecture Notes: J. Walt Oler Texas Tech University Concept of Stress Contents Concept of Stress
More informationFailure from static loading
Failure from static loading Topics Quiz /1/07 Failures from static loading Reading Chapter 5 Homework HW 3 due /1 HW 4 due /8 What is Failure? Failure any change in a machine part which makes it unable
More informationCoupling of plasticity and damage in glass fibre reinforced polymer composites
EPJ Web of Conferences 6, 48 1) DOI: 1.151/epjconf/1648 c Owned by the authors, published by EDP Sciences, 1 Coupling of plasticity and damage in glass fibre reinforced polymer composites R. Kvale Joki
More informationCOMPUTER AIDED DESIGN IN CASE OF THE LAMINATED COMPOSITE MATERIALS
6 th International Conference Computational Mechanics and Virtual Engineering COMEC 15 1516 October 15, Braşov, Romania COMPUER AIDED DESIGN IN CASE OF HE LAMINAED COMPOSIE MAERIALS Camelia Cerbu ransilvania
More informationUSE OF FINITE ELEMENT METHOD TO EVALUATE THE STRENGTH RESPONSE OF NOTCHED COMPOSITE LAMINATES UNDER TENSION ARJUN KOTHIDAR
USE OF FINITE ELEMENT METHOD TO EVALUATE THE STRENGTH RESPONSE OF NOTCHED COMPOSITE LAMINATES UNDER TENSION By ARJUN KOTHIDAR A thesis submitted in partial fulfillment of the requirements for the degree
More informationSamantha Ramirez, MSE. Stress. The intensity of the internal force acting on a specific plane (area) passing through a point. F 2
Samantha Ramirez, MSE Stress The intensity of the internal force acting on a specific plane (area) passing through a point. Δ ΔA Δ z Δ 1 2 ΔA Δ x Δ y ΔA is an infinitesimal size area with a uniform force
More informationFRACTURE TOUGHNESS OF ADHESIVE BONDED COMPOSITE JOINTS UNDER MIXED MODE LOADING.
FRACTURE TOUGHNESS OF ADHESIVE BONDED COMPOSITE JOINTS UNDER MIXED MODE LOADING. X. J. Gong, F. Hernandez, G. Verchery. ISAT  Institut Supérieur de l Automobile et des Transports, LRMA  Laboratoire de
More informationDESIGN OF LAMINATES FOR INPLANE LOADING
DESIGN OF LAMINATES FOR INPLANOADING G. VERCHERY ISMANS 44 avenue F.A. Bartholdi, 72000 Le Mans, France Georges.Verchery@m4x.org SUMMARY This work relates to the design of laminated structures primarily
More informationDynamic analysis of Composite Micro Air Vehicles
Dynamic analysis of Composite Micro Air Vehicles Shishir Kr. Sahu Professor and Head, Civil Engineering, National Institute of Technology, Rourkela, India Email: sksahu@nitrkl.ac.in ABSTRACT The present
More informationMECHANICS OF MATERIALS
CHATR Stress MCHANICS OF MATRIALS and Strain Axial Loading Stress & Strain: Axial Loading Suitability of a structure or machine may depend on the deformations in the structure as well as the stresses induced
More information